**Critical current in semiconductor nanowire**

**Josephson junctions in the presence of magnetic field**

**Tomohiro Yokoyama***1,2***, Mikio Eto**3**, and Yuli V. Nazarov**1

1 _{Kavli Institute of Nanoscience, Delft University of Technology, Delft, The Netherlands}
2

Center for Emergent Matter Science, RIKEN Institute, Wako, Japan

3 _{Faculty of Science and Technology, Keio University, Yokohama, Japan}

E-mail: [email protected]

**Abstract.** We study theoretically the critical current in semiconductor nanowire Josephson
junction with strong spin-orbit interaction. The critical current oscillates with an external
magnetic field. We reveal that the oscillation of critical current depends on the orientation of
magnetic field in the presence of spin-orbit interaction. We perform a numerical simulation
using a tight-binding model. The Andreev levels are calculated as a function of phase diﬀerence

*φ between two superconductors. The DC Josephson current is evaluated from the Andreev*

levels in the case of short junctions. The spin-orbit interaction induces the eﬀective magnetic
field. When the external field is parallel with the eﬀective one, the critical current oscillates
*accompanying the 0-π like transition at the cusp of critical current. The distance of cusps*
increases gradually with increasing of the angle between the external and eﬀective fields. The
magnetic anisotropy of critical current is attributed to the spin precession due to the spin-orbit
interaction.

**1. Introduction**

The spin-orbit (SO) interaction has attracted a lot of interest. In narrow-gap semiconductors, such as InAs and InSb, the strong SO interaction has been reported and many phenomena based on the SO interaction are investigated intensively, e.g., spin Hall eﬀect [1]. The SO interaction has a great advantage also for application to the spintronic devices and to quantum information processing. InAs and InSb nanowires are interesting nanostructure for the application and studied in recent experiments, e.g., the electrical manipulation of single electron spin in quantum dots fabricated on the nanowires [2]. Nanowire-superconductor hybrid systems have been also examined to investigate the Majorana fermions induced by the SO interaction and the Zeeman eﬀect [3].

*In Josephson junctions, the supercurrent flows when the phase diﬀerence φ between two*
superconductors is present. In this paper, we investigate theoretically the Josephson junction
of semiconductor nanowires with strong SO interaction. The supercurrent in semiconductor
nanowires has been reported by experiment groups [4, 5, 6, 7]. The Josephson eﬀect with SO
interaction has been studied theoretically for some materials, e.g., magnetic normal metals [8],
where the combination of SO interaction and exchange interaction results in an unconventional
*current-phase relation, I(φ) = I*0*sin(φ− φ0). The phase shift φ*0 deviates the ground state of

*junction from φ = 0 or π, which is so-called φ*0-state. The anomalous supercurrent is obtained

*at φ = 0. In previous studies, we have pointed out that the anomalous eﬀect is attributed*

*x*

### 0

_{L}

_{L}

*y*

**Figure 1.** Model for a semiconductor nanowire
Josephson junction. A tight-binding model is applied
to the normal region with hard-wall potentials forming
the nanowire. The nanowire is represented by a
*quasi-one dimensional system along the x direction. The*
*normal region is 0 < x < L and the superconducting*
*region induced by the proximity eﬀect is x < 0, x > L.*

to the spin-dependent channel mixing due to the SO interaction [9, 10]. In the present study, we focus on the critical current oscillation when an external magnetic field is applied. The DC Josephson current is evaluated from the Andreev levels in the case of short junction. We examine a numerical calculation using a tight-binding model for the nanowire. In this model, a particular form of SO interaction can be considered. When the angle between the external field and an eﬀective magnetic field due to the SO interaction is smaller, the oscillation period of critical current is shorter.

**2. Model**

*The nanowire along the x direction is connected to two superconductors (Fig. 1). At x < 0*
*and x > L, the superconducting pair potential is induced into the nanowire by the proximity*
*eﬀect. We assume that the pair potential is ∆(x) = ∆*0e*iφ/2* *at x < 0 and ∆(x) = ∆*0e*−iφ/2* at

*x > L, where φ is the phase diﬀerence between the two superconductors. In the normal region at*

*0 < x < L, ∆(x) = 0. When a magnetic field is applied to the junction, the Zeeman eﬀect is taken*
into account in the nanowire. The magnetic field is not too large to break the superconductivity
*and screened in the superconducting regions. The Hamiltonian is given by H = H*0*+ H*SO*+ H*Z

*with H*0 * = p*2

*/2m + Vconf*

*+ V*imp

*, the Rashba interaction H*SO

*= (α/¯h)(pyσ*ˆ

*x− pxσ*ˆ

*y*), and the

*Zeeman term H*Z

*= gµ*B

**B****· ˆσ/2, using eﬀective mass m, g-factor g (< 0 for InSb), Bohr magneton***µB*, and Pauli matrices ˆ

*conf*

**σ. We neglect the orbital magnetization eﬀect in the nanowire. V***describes the confining potential forming the nanowire. V*imp represents the impurity potentials.

We consider short junction, where the spacing between two superconductors is much smaller
*than the coherent length in the normal region, L≪ ξ. There is no potential barrier at x = 0, L.*
*The Zeeman energy E*Z =*|gµBB| and the pair potential ∆0* are much smaller than the Fermi
*energy E*F.

The Bogoliubov-de Gennes (BdG) equation is written as

(
*H− EF* ∆ˆ
ˆ
∆*†* *−(H∗− EF*)
) (
* ψ*e

*h )*

**ψ***= E*(

*e*

**ψ***h ) (1)*

**ψ**with ˆ*∆ = ∆(x)ˆ g. ψ*e

*= (ψ*e+

*, ψ*e

*−*)T

*h*

**and ψ***= (ψ*h+

*, ψ*h

*−*)T are the spinors for electron and hole,

respectively. ˆ*g =−iˆσy. The energy E is measured from the Fermi level E*F. The BdG equation

*determines the Andreev levels En* (*|En| < ∆0) as a function of φ.*

*The ground state energy of junction is given by E*gs*(φ) =* *−(1/2)*
∑

*n′En(φ), where the*
*summation is taken over all the positive Andreev levels, En(φ) > 0. The contribution from*
continuous levels (*|E| > ∆0*) can be disregarded in the case of short junctions [11]. At zero
*temperature, the supercurrent is calculated as I(φ) = (2e/¯h)(dEgs/dφ).* The current is a
periodic function for *−π ≤ φ < π. The maximum (or absolute value of minimum) of I(φ)*
*yields the critical current I*c.

The BdG equation in eq. (1) is expressed in terms of the scattering matrix [11]. The scattering
matrix of electrons (holes) transport in the normal region is given by ˆ*S*e ( ˆ*S*h). ˆ*S*e and ˆ*S*h are

### 0

### π

### 2π

### 0

### π

_{2π}

_{3π}

### 0

### π

_{/2}

### (a)

### (b)

### 0

### π

_{2π}

_{3π}

### 0

### π

* Figure 2. Numerical results of phase diﬀerence φ*0 at the minimum of ground-state energy

*when the number of conduction channel is unity and l*mfp*/L = 1.* The SO interaction is
*lSO/L = 0.2. The results are for a sample. (a) Grayscale plot of φ0* in the plane of magnetic
*field θB= E*Z*L/(¯hv*F*) and its direction θ. (b) Cross section of panel (a) at θ = 0.5π (solid), 0.3π*

*(broken), 0.15π (dotted), and 0 (dotted broken lines).*

related to each other by ˆ*S*e= ˆ*S*h*∗* for the short junctions. We denote ˆ*S*e= ˆ*S and ˆS*h = ˆ*S∗*. The

*Andreev reflection at x = 0 and L is described by the scattering matrix ˆr*he for the conversion

from electron to hole and ˆ*r*eh for that from hole to electron. The normal reflection can be

neglected. The matrix coeﬃcients of ˆ*r*he and ˆ*r*eh, e.g., exp*{−i arccos(E/∆0*)*− iφ/2} for ˆr*he at
*x = 0, are calculated from the boundary condition at x = 0 and L. The SO interaction does*

*not aﬀect the Andreev reflection coeﬃcients. The Andreev levels, En(φ), are obtained from the*
product of ˆ*S, ˆr*he, and ˆ*r*eh,

det(ˆ1*− ˆrehS*ˆ*∗*ˆ*r*he*S*ˆ
)

*= 0.* (2)

Equation (2) is equivalent to the BdG equation (1).

To calculate the scattering matrix ˆ*S, we adopt the tight-binding model which discretizes*

*a two-dimensional space (xy plane). The edges of nanowire are represented by a hard-wall*
*potential. The width of nanowire is W = 12a with the lattice constant a = 10nm. The Fermi*
*wavelength is fixed at λ*F *= 18a, where the number of conduction channels is unity. The length*

*of normal region is L = 50a. The on-site random potential by impurities is taken into account,*
the distribution of which potential is uniform. We set that the mean free path due to the
*impurity scattering is l*mfp*/L = 1. The SO length is l*SO*/L = 0.2 with l*SO *= k−1α* = ¯*h*2*/(mα).*
**The magnetic field is B = Be**θ*with the angle θ from the x axis in the xy plane.*

**3. Results**

We consider a sample for the nanowire. For the magnetic field, we introduce a parameter,

*θB= E*ZL/(¯*hvF*), which means an additional phase due to the Zeeman eﬀect in the propagation
*of electron and hole. Here, v*F is the Fermi velocity in the absence of SO interaction.

*Figure 2 shows the phase diﬀerence φ*0 *at the minimum of E*gs when the magnetic field is

*increased and rotated. In the absence of SO interaction, φ*0 *takes only 0 or π exactly and*

*clear 0-π transition happens (see Ref. [10]). In the presence of SO interaction, φ*0 is deviated

*from 0 and π, where the anomalous Josephson current is obtained. When the magnetic field*
*is in the y direction (θ = π/2), the transition between φ*0 *≈ 0 and φ0* *≈ π takes place around*
*θB* *= π/2, 3π/2,· · ·. The transition points are shifted gradually to large θB* with decreasing of

### 0

### π

_{2π}

_{3π}

### 0

### 1

### π

_{/2}

_{0}

### (a)

### (b)

* Figure 3. Numerical results of critical current I*c

*when N = 1 and l*mfp/L = 1. The SO

*interaction is l*SO*/L = 0.2. I0* *≡ e∆0/¯h. The sample is the same as that in Fig. 2. (a) Ic* as a

*function of magnetic field θB* *= E*Z*L/(¯hv*F*) when θ = 0.5π (solid), 0.3π (broken), 0.15π (dotted),*

*and 0 (dotted broken lines). (b) I*c*as a function of magnetic field orientation θ when θB= π/2*
*(solid), π (broken), and 2π (dotted lines).*

*angle θ. At θ≈ 0, the transition is not observed in Fig. 2.*

The transition points correspond to the positions of cusps of critical current. Figure 3(a)
*exhibits the critical current when the magnetic field increases. The critical current I*c oscillates

*as a function of θB*. The distance of cusps becomes long when the direction of magnetic field is
*tilted from the y axis. In the case of the parallel magnetic field to the nanowire (θ = 0), I*c has

*no cusp in accordance with no transition. The critical current at θ = 0 decreases with increase*
*of θB* *although φ*0 *is almost fixed at zero in Fig. 2(b). Figure 3(b) shows I*c when the magnetic

*field is rotated in the xy plane. The strength of magnetic field is fixed. We find the transition*
*with the angle θ in Fig. 2(a). The critical current also oscillates as a function of θ. At small*
*magnetic field (θB* *< π/2), Ic* *changes monotonically. The oscillation with θ can be obtained*
*when the magnetic field is θB* *> π/2. If the state of junction at θ = π/2 is φ*0 *≈ π (0), the*

critical current shows one cusp (two cusps) in Fig. 3(b). Therefore we can estimate the state at

*θ = π/2 from the magnetic anisotropy of critical current.*

**4. Conclusions and Discussion**

We have studied the DC Josephson eﬀect in the semiconductor nanowire with strong SO
interaction. We have examined a numerical simulation using the tight-binding model in the case
of short junction. The combination of SO interaction and Zeeman eﬀect in the nanowire results
in the anomalous Josephson eﬀect. The critical current oscillates as a function of magnetic field.
In the presence of SO interaction, the oscillation of critical current depends on the magnetic
field orientation. The oscillation period is the shortest when the magnetic field is perpendicular
*to the nanowire. For a parallel magnetic field to the nanowire, the 0-π (like) transition and the*
cusp of critical current are not found.

In this numerical model, we have considered the Rashba interaction. In the quasi-one-dimensional nanowire, the eﬀective magnetic field induced by the Rashba interaction is in the

*y direction. The magnetic anisotropy of critical current is understood intuitively by the spin*

precession in the propagation of electron and hole. When the external magnetic field is parallel
*to the eﬀective SO field (the y direction), the spin quantization axis is fixed in that direction.*
The electron and hole receive the additional phase in the propagation. On the other hand, when

*the external field is in the x direction, the spin quantization axes for electron and hole are not*
parallel with each other since the eﬀective fields for electron and hole are antiparallel. The spin
of electron and hole forming the Andreev bound state is rotated, which rotation cancels out the
*phase θB* due to the Zeeman splitting. As a result, the critical current oscillation disappears.
*In the case of general SO interaction, the eﬀective field would be deviated from the y axis. By*
measuring the magnetic anisotropy of critical current oscillation, we can evaluate the direction
of eﬀective field due to the SO interaction.

**Acknowledgments**

We acknowledge financial support by the Motizuki Fund of Yukawa Memorial Foundation. We acknowledge fruitful discussions about experiments with Professor L. P. Kouwenhoven, A. Geresdi, V. Mourik, K. Zuo of Delft University of Technology. T.Y. is a JSPS Postdoctoral Fellow for Research Abroad.

**References**

**[1] Kato Y K, Myers R C, Gossard A C, and Awschalom D D 2004 Science 306 1910**

[2] Nadj-Perge S, Pribiag V S, van den Berg J W G, Zuo K, Plissard S R, Bakkers E P A M, Frolov S M, and
**Kouwenhoven L P 2012 Phys. Rev. Lett. 108 166801**

**[3] Mourik V, Zuo K, Frolov S M, Plissard S R, Bakkers E P A M, and Kouwenhoven L P 2012 Science 336 1003***[4] Doh Y-J, van Dam J A, Roest A L, Bakkers E P A M, Kouwenhoven L P, and Franceschi S De 2005 Science*

**309 272**

[5] Gharavi K, Holloway G W, Haapamaki C M, Ansari M H, Muhammad M, LaPierre R R, and Baugh J arXiv: 1405.7455

[6] Li C, Kasumov A, Murani A, Sengupta S, Fortuna F, Napolskii K, Koshkodaev D, Tsirlina G, Kasumov Y, Khodos I, Deblock R, Ferrier M, Gu´eron S, and Bouchiat H arXiv: 1406.4280

[7] Kouwenhoven L P, Geresdi A, Mourik V, and Zuo K (private communications)
**[8] Buzdin A 2008 Phys. Rev. Lett. 101 107005**

**[9] Yokoyama T, Eto M, and Nazarov Yu V 2013 J. Phys. Soc. Jpn. 82 054703****[10] Yokoyama T, Eto M, and Nazarov Yu V 2014 Phys. Rev. B 89 195407**